refractive-index matching between liquid crystals and photopolymers
Embed Size (px)
Refractive-index matching between liquid crystals and photopolymers
Jun LiGreg BairdYi-Hsin LinHongwen RenShin-Tson Wu
Abstract — Refractive indices of two photocurable polymers, NOA65 and NOA81 (Norland OpticalAdhesive), and two series of Merck liquid crystals, E-series (E44, E48, and E7) and BL-series (BL038,BL003 and BL006), and two UCF high-birefringence liquid-crystal mixtures were measured using anAbbe refractometer in the visible spectral region and 15–55°C temperature range. Some liquid crystalshave excellent index matching with NOA65 in the red, while some fit better in the blue spectral region.To validate this index-matching property found in the material level, we prepared some polymer-dis-persed liquid-crystal devices. Good correlations between material and device performances areobtained.
Keywords — Liquid crystals, Norland polymers, refractive index, polymer-dispersed liquid crystals.
1 IntroductionPolymer-dispersed liquid crystal (PDLC) and polymer-sta-bilized liquid crystal (PSLC) are useful for displays,1–4 tun-able wavelength filters,5–7 tunable liquid-crystal lenses,8,9
and polarization-independent phase modulators.10 In aPDLC, the refractive-index difference between the LCdroplets and polymer matrix plays an important role in de-termining the voltage-off and voltage-on state transmit-tance. In a normal-mode PDLC, the droplet size iscontrolled at ~1 μm, which is comparable with the visible-light wavelength. In the voltage-off state, the droplets arerandomly oriented. The index mismatch between the LC(whose average refractive index is given by ⟨n⟩ = (ne +2no)/3) and polymer matrix (np) affects the light-scatteringcapability. For a given droplet size, the larger the index mis-match, the higher the light scattering. Conversely, in thevoltage-on state the LC directors inside the droplets are reori-ented along the electric-field direction so that the refractiveindex becomes no; the ordinary refractive index. If no ~ np,then the PDLC becomes isotropic and will have an excellenttransmittance. Therefore, the preferred LC material forPDLC is not only high birefringence (Δn = ne – no) but alsogood index match between no and np. In a PSLC system,polymer networks help to improve response time.11 A goodindex match would reduce light scattering.
In this paper, we compare the refractive index of curedpolymers with liquid crystals at different wavelengths andtemperatures. In Section 2, the fabrication method of thethin cured polymer films is briefly described. The refractiveindex of the cured polymer films (NOA65 and NOA81) andsix nematic liquid crystals (BL038, BL006, BL003, E48,E44, and E7) were measured using a multi-wavelengthAbbe refractometer. In Section 3, we compare the refractiveindex between NOA 65 and these six commercial liquidcrystals, and NOA81 with two UCF high birefringence mix-tures: UCF-1 and UCF-2. In Section 4, we fabricate somePDLC cells using the four selected index-matched LC mix-
tures in the NOA65 polymer system and characterize theirelectro-optic properties at λ = 633 nm. In Section 5, weobtain good correlation between material and device per-formances.
2 Measurements of refractive indicesNOA65 (Norland Optical Adhesive) is a commonly usedphotocurable polymer because its refractive index (np ~1.52) is close to the no of many commercial LC mixtures. Onthe other hand, NOA81 has a higher refractive index (np ~1.56), which is close to the no of our UCF high-birefrin-gence LC mixtures. In this study, we compare the refractiveindices of NOA65 with six Merck LC mixtures, and NOA81with two UCF high birefringence LC mixtures using a mul-tiwavelength Abbe refractometer (Atago DR-M4). BeforeUV curing, NOA65 and NOA81 are clear and colorless liq-uids. The measurement of the monomers is fairly simple.However, in a practical device, such as a PDLC, all themonomers are cured to form a polymer matrix. Therefore,it is more meaningful to measure the refractive index of thecured polymers than the monomers.
In order to fabricate a polymer film, we infiltrated themonomers into an empty cell with a 1-mm gap using capil-lary flow. The cells were placed on a hot plate with a con-stant temperature (T ~ 50°C). Then, we illuminated the cellwith a uniform UV light (I = 14 mW/cm2, λ ~ 365 nm) for40 minutes because of the large cell gap. We then peeled offthe glass substrates and removed the thick polymer film undera high temperature (T ~ 120°C). The film was kept in a stovewith a constant temperature of 50°C for 12 hours to agecompletely. The cured polymer film of NOA65 is quite flex-ible, while the cured NOA81 is a little rigid. In order to getan accurate measurement, we cut the films into rectangularparallelepipeds of the following dimensions: 15 mm long, 9mm wide, and 1 mm thick. The bottom surface of the sam-ples was polished so that it made contact with the mainprism surface of the Abbe refractometer completely. First,
The authors are with the College of Optics and Photonics, University of Central Florida, Orlando, FL 32816, U.S.A.; telephone 407/823-4763,fax 407/823-6880, e-mail: [email protected].
© Copyright 2005 Society for Information Display 1071-0922/05/1312-1017$1.00
Journal of the SID 13/12, 2005 1017
we put a small drop of contact liquid (monobromo-naphthalene) on the main prism, then put the sample on andensured the contact liquid spread evenly between the sam-ple and the main prism. It is important to get rid of any dustand bubbles between the solid sample and the main prism.A lighting glass was used to compensate for the weak lightbecause the samples are thin. Similarly, we spread a smallamount of the contact liquid on the top surface of the sam-ple and put the lighting glass on top of the contact liquid.The thin contact liquid should spread evenly between thesample and the lighting glass. Now the contact liquid issandwiched as films between the main prism and the sampleand between the sample and the lighting glass. The incidentlight entered the sample slightly aslant from the upside.
Figure 1 shows the experimental setup for measuringthe cured polymer films. By moving the lighting glass to thefront and rear, pressing the lighting glass to the sample byfingers, and adjusting the height and angle of the lightguide, we found a clear and correct boundary line. This isthe sign for the accurate measurements using the Abbe refrac-tometer. We measured the refractive indices of LCs andpolymers at six wavelengths: 450, 486, 546, 589, 633, and656 nm. By connecting a constant circulating temperaturebath (Atago 60-C3) with the Abbe refractometer, we meas-
ured the temperature-dependent refractive index of thesamples from 15 to 55°C at 5°C intervals.
Figure 2 shows the wavelength- and temperature-dependent refractive index of the cured NOA65 polymer.The squares, circles, upward triangles, downward triangles,diamonds, and pentagons represent the measured refractiveindex of NOA65 at λ = 450, 486, 546, 589, 633, and 656 nm,respectively. In Fig. 2, we find the refractive index ofNOA65 decreases linearly as temperature increases at agiven wavelength:
n(T) = A – BT, (1)
where the A and B coefficients in Eq. (1) are constant at agiven wavelength. The fitting values of A and B are listed inTable 2. This linear decrease with increasing temperaturemight be related to the isotropic nature of NOA65. As thetemperature increases, the density of most of the isotropic
FIGURE 1 — The experimental setup for measuring the refractive indexof cured polymer films: NOA65 and NOA81.
FIGURE 2 — Wavelength- and temperature-dependent refractive indexof cured NOA65. The squares, circles, upward triangles, downwardtriangles, diamonds, and pentagons represent the measured refractiveindex of NOA65 at λ = 450, 486, 546, 589, 633, and 656 nm,respectively. Solid lines are fittings using Eq. (1) and the fitting parametersare listed in Table 1.
TABLE 1 — The measured refractive index of cured NOA65 film at λ =450, 486, 546, 589, 633, and 656 nm at different temperatures. TABLE 2 — The fitting parameters for the refractive index [Eq. (1)] of
NOA65 and NOA81 at λ = 450, 486, 546, 589, 633, and 656 nm.
1018 Li et al. / Refractive-index matching between LCs and photopolymers
organics decreases which, in turn, causes the refractive in-dex to decrease linearly.
Figure 3 shows a similar plot for NOA81. The squares,circles, upward triangles, downward triangles, diamonds,and pentagons represent the measured refractive index ofNOA81 at λ = 450, 486, 546, 589, 633, and 656 nm, respec-tively. Similarly to NOA65, the refractive index of NOA81decreases linearly as the temperature increases. The solidlines in Fig. 3 are fittings using Eq. (1) and the fittingparameters are listed in Table 2. We also measured thewavelength- and temperature-dependent refractive index ofNOA65 and NOA81 in the monomer state. After UV curing,the refractive index of the cured polymers increases 1.7%and 2.2% for NOA65 and NOA81, respectively. This slightrefractive-index increase originates from the increased den-sity of the polymer after cross-linking.
For a normal-mode PDLC, the light scattering in thevoltage-off state depends on the LC birefringence; thehigher the birefringence, the higher the scattering effi-ciency. In the voltage-on state, the transmittance dependson the refractive index match between the LC (no) and thepolymer matrix (np). If no ~ np, then the on-state will behighly transparent. After having measured the np of NOA65,
we selected two commercial high birefringence LC serieswith their no close to np. The two LC series are BL-series(BL038, BL006, and BL003) and E-series (E48, E44, andE7). To measure the refractive indices, we aligned the LCsperpendicular to the main and secondary prism surfaces ofthe Abbe refractometer by coating these two surfaces witha surfactant comprising of 0.294 wt.% hexadecyletri-methyle-ammonium bromide (HMAB) in methanol solu-tion. The measured extraordinary (ne) and ordinary (no)refractive indices of E48, E44, E7, BL038, BL006, andBL003 are listed in Tables 5–10, respectively. From thisdata, we find that ne always decreases as temperature increases,whereas no declines modestly first and then increases afterthe temperature passes the crossover temperature.12 Theaverage refractive index ⟨n⟩ [which is defined as (ne + 2no)/3]also decreases linearly as temperature increases.13
The wavelength-dependent refractive index of theUV-cured polymers can be described by the extendedCauchy equation,14–16
Here, A, B, and C are Cauchy coefficients which are con-stant at a given temperature.
3 Refractive-index comparisonsNOA81 (np ~ 1.56) has a higher refractive index thanNOA65 (np ~ 1.52). For a linearly conjugated LC, a high nooften leads to a high Δn. Most of the commercially available
n AB C
( ) .ll l
= + +2 4
FIGURE 3 — Wavelength- and temperature-dependent refractive indexof cured NOA81. The squares, circles, upward triangles, downwardtriangles, diamonds, and pentagons represent the measured refractiveindex of NOA81 at λ = 450, 486, 546, 589, 633, and 656 nm,respectively. Solid lines are fittings using Eq. (1) and the fitting parametersare listed in Table 3.
TABLE 3 — The measured refractive index of cured NOA81 film at λ =450, 486, 546, 589, 633, and 656 nm at different temperatures.
TABLE 4 — The fitting parameters for the refractive index [Eq. (2)] of NOA65 and NOA81 and the ordinary refractive index of E48, E44,E7, BL038, BL006, BL003, UCF-1, and UCF-2 at _ = 20°C.
Journal of the SID 13/12, 2005 1019
high birefringence (Δn ~ 0.20–0.28) liquid crystals haveno ~ 1.50–1.52. These are the mixtures of cyano-biphenylsand cyano-terphenyls, e.g., Merck E-series and BL-series.Only some high birefringence (Δn = 0.4) LCs have no >1.55. These are mainly isothiocyanato-tolane mixtures, e.g.,UCF-series. Thus, we compare the index matching of someMerck E-series (E7, E48, and E44) and BL-series (BL003,BL006, and BL038) liquid crystals with NOA65, and somehigh birefringence UCF mixtures (UCF-1 and UCF-2) withNOA81.
Figure 4 shows the measured refractive index of theUV-cured NOA65 and the ordinary refractive index of E48,E44, and E7, as a function of wavelength at T = 20°C. Thefilled circles, open squares, upward triangles, and down-
ward triangles are the measured ordinary refractive index ofNOA65, E48, E44, and E7, respectively. The respectivesolid lines represent the fittings of each material using theextended Cauchy model [Eq. (2)]. The fitting parameters A,B, and C are listed in Table 4. From Fig. 4, E48, E44, andE7 all have a reasonably good index matching with NOA65.The mismatch is within 0.005 at λ = 550 nm. More specifi-cally, E44 has the best match in the red spectral region whileE7 and E48 have the best match in the blue region. In thegreen region (λ = 546 nm), E44 has a slightly higher index,while E7 and E48 are slightly lower than NOA65, but thedifference is in the third decimal.
Figure 5 shows the refractive index of the curedNOA65 and the ordinary refractive index of BL038, BL006,
TABLE 5 — The measured refractive indices (ne and no) of E48 at λ = 450, 486, 546, 589, 633, and 656 nm at different temperatures.
TABLE 6 — The measured refractive indices (ne and no) of E44 at λ = 450, 486, 546, 589, 633, and 656 nm at different temperatures.
1020 Li et al. / Refractive-index matching between LCs and photopolymers
and BL003 as a function of wavelength at T = 20°C. Thefilled circles, open squares, upward triangles, and down-ward triangles are the measured ordinary refractive index ofNOA65, BL038, BL006, and BL003, respectively. The solidlines represent the fittings of each material using the extendedCauchy model [Eq. (2)]. The fitting parameters are listed inTable 4. In Fig. 5, BL038, BL006, and BL003 have a similartrend in no(λ). The index matching with NOA65 is prettygood in the green and red spectral regions. A larger devia-
tion is observed in the blue region, but the difference is stillin the third decimal.
The ordinary refractive index of NOA81 is larger thanNOA65. The measured value of NOA81 at λ = 589 nm andT = 20°C is 1.5662. No commercially available LC mixtureshave such a high no. We have formulated two new LC mixturesdesignated as UCF-1 and UCF-2 whose ordinary refractiveindex matches with NOA81. Figure 6 shows the refractiveindex of the cured NOA81 and the ordinary refractive indexof UCF-1 and UCF-2 as a function of wavelength at T =20°C. The filled circles, open squares, and upward triangles
TABLE 7 — The measured refractive indices (ne and no) of E7 at λ = 450, 486, 546, 589, 633, and 656 nm at different temperature.
FIGURE 5 — Wavelength-dependent refractive index of NOA65 and theordinary refractive index of BL038, BL006, and BL003 at T = 20°C. Theopen squares, upward triangles, filled circles, and downward trianglesare the measured refractive index of BL038, BL006, NOA65 and BL003,respectively. The solid lines represent the fittings using the extendedCauchy model [Eq. (2)]. The fitting parameters are listed in Table 4.
FIGURE 4 — Wavelength-dependent refractive index of NOA65 and theordinary refractive index of E48, E44 and E7 at T = 20°C. The opensquares, upward triangles, filled circles, and downward triangles are themeasured refractive index of E48, E44, NOA65 and E7, respectively. Thesolid lines represent the fittings using the extended Cauchy model [Eq.(2)]. The fitting parameters are listed in Table 4.
Journal of the SID 13/12, 2005 1021
are the measured ordinary refractive index of NOA81,UCF-1, and UCF-2, respectively. The solid lines representthe fittings of each material using the extended Cauchymodel [Eq. (2)]. The fitting parameters are listed in Table 4.In Fig. 6, the no of UCF-1 and UCF-2 match well with thatof NOA81 in the red region. As the wavelength gets shorter,the deviation increases gradually. This is because the longestelectronic absorption band of the high birefringence LCsusually extends to λ2 ~ 350-nm region.17 In the blue spec-tral region, the resonance effect to the refractive index ismore pronounced because the wavelength is closer to λ2.
In a PDLC system, good index matching (no ~ np)between the employed polymer and liquid crystal helps toimprove the transmittance in the voltage-on state. On theother hand, a larger index mismatch (⟨n⟩ > np), i.e., a higherbirefringence LC enhances the light-scattering efficiency inthe voltage-off state. However, refractive-index match ormismatch is not the only factor deciding the PDLCperformance. UV stability of liquid crystals and miscibilitybetween polymers and liquid crystals also play importantroles affecting the PDLC properties. As we discussedbefore, the E-series and BL-series liquid crystals all have agood index match with NOA65. All these six liquid crystalsare good candidates for PDLC application when NOA65 isused. In the visible spectrum, E48 and E7 have very similarordinary refractive index at T = 20°C, as do BL038 andBL003. However, E48 (BL038) has a higher birefringencethan E7 (BL003). Thus, we choose to compare the NOA65PDLC systems using BL038, E48, BL006, and E44.
4 PDLC cell fabrication and measurementsTo prepare PDLC samples, we mixed NOA65 with E48,E44, BL038, and BL006; each at a 30:70 wt.% ratio. To ensurea uniform mixing, we stirred the LC/monomer mixtures usingsmall magnetic stirrers for half an hour at T = 120°C. EachLC/monomer mixture was then injected to an empty glasscell (cell gap ~8 μm) in the isotropic state. The inner sur-faces of the glass substrates were coated with a thin indium-tin-oxide layer, but no polyimide layer. To cure the samples,the cells were exposed to UV light (I = 65 mW/cm2, λ ~ 365nm) for 15 minutes at T = 20°C.
The voltage-dependent transmittance (VT) curveswere measured and used to compare the contrast ratio ofthe PDLC cells. The experimental setup is shown in Fig. 7.
FIGURE 6 — Wavelength-dependent refractive index of NOA81 and theordinary refractive index of UCF-1 and UCF-2 at T = 20°C. The filledcircles, open squares, and upward triangles are the measured refractiveindex of NOA81, UCF-1, and UCF-2, respectively. The solid linesrepresent the fittings using the extended Cauchy model [Eq. (2)]. Thefitting parameters are listed in Table 11.
TABLE 8 — The measured refractive indices (ne and no) of BL038 at λ = 450, 486, 546, 589, 633, and 656 nm at different temperature.
1022 Li et al. / Refractive-index matching between LCs and photopolymers
An unpolarized He-Ne laser (λ = 633 nm) beam was nor-mally incident on the PDLC cell. A photodiode detector wasplaced at 25 cm behind the cell. The corresponding collec-tion angle is ~2°. A LabVIEW data acquisition system wasused to control the applied voltage and record the measuredVT curves.
5 Results and discussionFrom the measured VT curves, we find that BL038 is betterthan BL006, and E48 is better than E44 in the NOA65PDLC systems, although these four LC mixtures all have agood index match with NOA65. The BL038 PDLC and E48PDLC cells exhibit a lower transmittance in the voltage-offstate and a higher transmittance in the voltage-on state thanthat of BL006 PDLC and E44 PCLC cells, respectively. Itimplies that the refractive index match is not the only factoraffecting the contrast ratio of a PDLC; the LC/polymer mis-cibility also plays an important role. It is likely that BL038
and E48 have a better miscibility in NOA65 than BL006 andE44.
In Fig. 8, we compare the normalized VT curves of theBL038 and E48 PDLC cells at λ = 633 nm. For both cells,the polymer (NOA65) and LC ratio is 30:70 and cell gap is8 μm. To calibrate the substrate reflection losses, the trans-mittance of the PDLC cell is normalized to that of a homo-geneous cell filled with the corresponding liquid crystal.The red line represents the transmittance of the BL038PDLC cell and the blue line represents the transmittance ofthe E48 PDLC cell. In Fig. 8, the BL038 PDLC cell has alower transmittance at V = 0 and a higher transmittance in
FIGURE 7 — The experimental setup for measuring the transmittance ofthe PDLC cells.
TABLE 9 — The measured refractive indices (ne and no) of BL006 at λ = 450, 486, 546, 589, 633, and 656 nm at different temperature.
FIGURE 8 — Voltage-dependent normalized transmittance of the BL038and E48 PDLC cells at λ = 633 nm. For both cells, the LC:NOA65 ratiois 70:30. The two cells have same thickness (d = 8 μm) and have nopolyimide layer on the glass substrates.
Journal of the SID 13/12, 2005 1023
the on-state than E48. The saturation voltage of both cellshappens at ~20 Vrms, thus, we define the contrast ratio as:CR = T (V = 20 Vrms)/T (V = 0). The measured contrast ratiois 13:1 and 10:1 for the BL038 and E48 PDLC cells, respec-tively. We could enhance contrast ratio by using a thickercell gap. The tradeoff is the increased operating voltage.
Two factors contributing to the higher contrast ratio ofthe BL038 PDLC cell over E48 are higher birefringenceand better index matching with NOA65. In Fig. 9, we com-pare the wavelength-dependent refractive index of NOA65and the ordinary refractive index of BL038 and E48 at T =20°C. The filled circles, open squares, and upward triangles
are the measured refractive index of NOA65, BL038, andE48, respectively. The solid lines represent the fittings usingthe extended Cauchy model [Eq. (2)]. The fitting parame-ters are listed in Table 4. From Fig. 9, we find that BL038has a better index match than E48 at λ = 633 nm. Thus, theBL038 PDLC cell has a higher transmittance in the voltage-on state than the E48 cell when the He–Ne laser (λ = 633nm) is used. However, this explanation is only qualitative. Inthe voltage-on state, the LC directors near the innerboundaries of the droplets are harder to be reoriented bythe electric field because of the surface anchoring effect.These anchored LC directors have some ne components. Asa result, the effective refractive index in the voltage-on state
FIGURE 9 — Wavelength-dependent refractive index of NOA65 (circles)and the ordinary refractive index of BL038 (squares) and E48 (triangles)at T = 20°C. The solid lines represent the fittings using the extendedCauchy model [Eq. (2)]. The fitting parameters are listed in Table 4.
TABLE 10 — The measured refractive indices (ne and no) of BL003 at λ = 450, 486, 546, 589, 633, and 656 nm at different temperature.
FIGURE 10 — Wavelength-dependent birefringence of BL038 (squares)and E48 (triangles) at T = 20°C. The solid lines are fittings using thesingle-band model [Eq. (3)]. The fitting parameters [G(μm–2), λ*(μm)] forBL038 and E48 are [3.509, 0.252] and [3.210, 0.244], respectively.
1024 Li et al. / Refractive-index matching between LCs and photopolymers
is slightly larger than no It is difficult to estimate how muchthese boundary layers contribute to the effective refractiveindex. It should be mentioned that the results shown inFig. 9 are for convenient demonstration only because of theavailability of a He–Ne laser light source. For practicalPDLC display, human eyes are more sensitive to green thanred. Therefore, the device should be optimized at a greenwavelength (λ ~ 550 nm).
Figure 10 shows the wavelength-dependent birefrin-gence of BL038 and E48 at T = 20°C. The squares and tri-angles represent the experimental data of BL038 and E48,respectively. The solid lines are fittings using the followingsingle-band birefringence dispersion model18:
where G is a proportionality constant and λ* is the meanresonant wavelength of the liquid crystal. The fitting pa-rameters [G (μm–2), λ* (μm)] for BL038 and E48 are[3.509, 0.252] and [3.210, 0.244], respectively. In Fig. 10,BL038 exhibits a larger birefringence than E48 in the entirevisible spectral region. Thus, the difference between the aver-age refractive index of BL038 and the refractive index ofNOA65 is larger than that between E48 and NOA65, i.e.,the refractive-index mismatch between BL038 and NOA65is larger than that between E48 and NOA65. A larger indexmismatch leads to a higher scattering efficiency. As a result,the BL038 PDLC cell has a lower transmittance at V = 0than the E48 cell.
The refractive index of cured polymers, NOA65 andNOA81, were measured at six visible wavelengths and in thetemperature range from 20 to 55°C using a multi-wave-length Abbe refractometer. The refractive indices of MerckE-series (E48, E44, and E7) and BL-series (BL038, BL006,and BL003) LC mixtures were measured. Comparativestudy on the refractive index between these liquid crystalsand cured polymers was made. Among the LC materials westudied, BL038 and E48 are good candidates for makingPDLC system incorporating NOA65. Indeed, the BL038PDLC cell shows a higher contrast ratio than the E48 cellbecause BL038 has a better-matched ordinary refractiveindex, higher birefringence, and similar miscibility as com-pared to E48. Liquid crystals having a good miscibility withpolymer, matched ordinary refractive index, and higherbirefringence help to improve the PDLC contrast ratio fordisplay applications.
References1 J L Fergason, “Polymer encapsulated nematic liquid crystals for display
and light control applications,” SID Symposium Digest Tech Papers 16,68–69 (1985).
2 J W Doane, A Golemme, B G Wu, and S Zumer, “Field controlled lightscattering from nematic microdroplets,” Appl Phys Lett 48, 269–271(1986).
3 P S Drzaic, Liquid Crystal Dispersions (World Scientific, Singapore,1995).
4 S T Wu and D K Yang, Reflective Liquid Crystal Displays (New York,Wiley, 2001).
5 S Matsumoto, M Houlbert, T Hayashi, and K Kubodera, “Fine dropletsof liquid crystals in a transparent polymer and their response to anelectric field,” Appl Phys Lett 69, 1044–1046 (1996).
6 S Matsumoto, K Hirabayashi, S Sakata, and T Hayashi, “Tunable wave-length filter using nano-sized droplets of liquid crystal,” IEEE Photon-ics Technol Lett 11, 442–444 (1999).
7 D E Lucchetta, R Karapinar, A Manni, and F Simoni, “Phase-onlymodulation by nanosized polymer-dispersed liquid crystals,” J ApplPhys 91, 6060–6065 (2002).
8 H Ren, Y H Fan and S T Wu, “Tunable Fresnel lens using nanoscalepolymer-dispersed liquid crystals,” Appl Phys Lett 83, 1515–1517(2003).
9 H Ren, Y H Fan, Y H Lin, and S T Wu, “Tunable-focus microlens arraysusing nanosized polymer-dispersed liquid crystal droplets,” Opt Com-mun 247, 101–106 (2005).
10 H Ren, Y H Lin, Y H Fan, and S T Wu, “Polarization-independentphase modulation using a polymer-dispersed liquid crystal,” Appl PhysLett 86, 141110 (2005).
11 Y H Fan, Y H Lin, H Ren, S Gauza, and S T Wu, “Fast-response timeand scattering-free polymer network liquid crystals for infrared lightmodulators,” Appl Phys Lett 84, 1233–1235 (2004).
12 J Li, S Gauza, and S T Wu, “High temperature-gradient refractiveindex liquid crystals,” Opt Express 12, 2002–2010 (2004).
13 J Li, S Gauza, and S T Wu, “Temperature effect on liquid crystalrefractive indices,” J Appl Phys 96, 19–24 (2004).
14 S T Wu, C S Wu, M Warenghem, and M Ismaili, “Refractive-indexdispersions of liquid-crystals,” Opt Eng 32, 1775–1780 (1993).
15 J Li and S T Wu, “Extended Cauchy equations for the refractive indicesof liquid crystals,” J Appl Phys 95, 896–901 (2004).
16 J Li and S T Wu, “Two-coefficient Cauchy model for low birefringenceliquid crystals,” J Appl Phys 96, 170–174 (2004).
17 S Gauza, C H Wen, N Janarthanan, C S Hsu, and S T Wu, “Super highbirefringence isothiocyanato biphenyl-bistolane liquid crystals,” Jpn JAppl Phys 43, 7634–7638 (2004).
18 S T Wu, “Birefringence dispersions of liquid crystals,” Phys Rev A 33,1270–1274 (1986).
Jun Li is a Ph.D. candidate at the College of Opticsand Photonics, University of Central Florida, Orlando,Florida. He received his B.S. degree in mechani-cal engineering and M.S. degree in automation,both from Tsinghua University, P. R. China. Hiscurrent research is to develop structure-propertycorrelation of liquid crystals, novel liquid-crystalmaterials with high dno/dT at room temperaturefor highly thermal tunable liquid-crystal photoniccrystal bandgap fibers, and measurements of liq-
uid-crystal refractive indices in the visible and infrared spectral regions.His future work will focus on the polymer-dispersed liquid crystal,microdisplay technology, and novel liquid crystals for display and pho-tonic applications.
Dn G( ) ,l l ll l
Journal of the SID 13/12, 2005 1025
Greg Baird is a junior at the University of Mis-souri-Rolla majoring in ceramic engineering. Hehas worked the past four years for a specialtyglass manufacturing company Mo-Sci. He hasbeen involved in many projects that include:crown cementation glass, NVIS glass, and glassmicrospheres among others. Outside of the class-room Greg has been involved in multiple compet-ing engineering teams. He was part of a designteam that took first place in the 2004 American
Ceramic Society’s annual ceramic putter competition, and also a teamthat received an honorable mention in the National Hydrogen Associa-tion’s 2004 hydrogen design contest. In 2005, Greg joined UCF for thesummer through the NSF-sponsored research experience for under-graduates program.
Yi-Hsin Lin is a Ph.D. candidate at the College ofOptics and Photonics, University of Central Florida,Orlando, Florida. She received her M.S. degree inelectro-optical engineering from National ChiaoTung University, and B.S. in physics from NationalTsinghua University, Taiwan. Her current researchis to develop novel polarization-independent liq-uid-crystal devices, novel liquid-crystal displays,and fast-response infrared phase modulators foroptical communications.
Hongwen Ren received his Ph.D. from Chang-chun Institute of Optics, Chinese Academy of Sci-ences, China. He joined the College of Opticsand Photonics, University of Central Florida as aresearch scientist in 2001. He is currently engagedin the research of liquid-crystal photonics for opticalcommunications, electrically tunable liquid-crys-tal lens and liquid lens for zoom lens applica-tions, and polymer-stabilized liquid crystals forfast-response polarization independent phasemodulators.
Shin-Tson Wu is a PREP Professor at the Collegeof Optics and Photonics, University of CentralFlorida. Prior to joining UCF in 2001, Dr. Wuworked at Hughes Research Laboratories (Malibu,California) for 18 years. He received his Ph.D.from the University of Southern California and hisB.S. in physics from National Taiwan University.His studies at UCF concentrate in foveated imag-ing, bio-photonics, optical communications, liq-uid-crystal displays, and liquid-crystal materials.
Dr. Wu is a Fellow of the IEEE, SID, and OSA. He has co-authored twobooks: Reflective Liquid Crystal Displays (Wiley, 2001) and Optics andNonlinear Optics of Liquid Crystals (World Scientific, 1993).
1026 Li et al. / Refractive-index matching between LCs and photopolymers